Phase Transitions and Coexistence of Magnetic and Electric Orders in the Methylhydrazinium Metal Formate Frameworks
Mączka, Mirosław; Gągor, Anna; Ptak, Maciej; Paraguassu, Waldeci; da Silva, Tercio Almeida; Sieradzki, Adam; Pikul, Adam; Chemistry of Materials 29 (2017) 2264–; doi:10.1021/acs.chemmater.6b05249

data_4002721
_publ_section_title
;
 Phase Transitions and Coexistence of Magnetic and Electric Orders in the
 Methylhydrazinium Metal Formate Frameworks
;
_journal_issue                   5
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2264
_journal_paper_doi               10.1021/acs.chemmater.6b05249
_journal_volume                  29
_journal_year                    2017
_chemical_formula_sum            'C8 H20 Mn2 N4 O12'
_chemical_formula_weight         474.16
_space_group_crystal_system      triclinic
_space_group_IT_number           1
_space_group_name_Hall           'P 1'
_space_group_name_H-M_alt        'P 1'
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                63.28(3)
_cell_angle_beta                 63.31(3)
_cell_angle_gamma                60.06(3)
_cell_formula_units_Z            1
_cell_length_a                   8.198(2)
_cell_length_b                   8.200(2)
_cell_length_c                   8.933(3)
_cell_measurement_reflns_used    1860
_cell_measurement_temperature    100.0(4)
_cell_measurement_theta_max      28.9230
_cell_measurement_theta_min      2.9810
_cell_volume                     444.8(3)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35h (release 09-02-2015 CrysAlis171 .NET)
(compiled Feb  9 2015,16:26:32)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35h (release 09-02-2015 CrysAlis171 .NET)
(compiled Feb  9 2015,16:26:32)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35h (release 09-02-2015 CrysAlis171 .NET)
(compiled Feb  9 2015,16:26:32)
;
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      100.0(4)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 10.6249
_diffrn_detector_type            Atlas
_diffrn_measured_fraction_theta_full 0.945
_diffrn_measured_fraction_theta_max 0.862
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Atlas'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0412
_diffrn_reflns_av_unetI/netI     0.0537
_diffrn_reflns_Laue_measured_fraction_full 0.945
_diffrn_reflns_Laue_measured_fraction_max 0.862
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            5320
_diffrn_reflns_point_group_measured_fraction_full 0.945
_diffrn_reflns_point_group_measured_fraction_max 0.862
_diffrn_reflns_theta_full        28.000
_diffrn_reflns_theta_max         29.232
_diffrn_reflns_theta_min         2.668
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    1.487
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.26827
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35h (release 09-02-2015 CrysAlis171 .NET)
(compiled Feb  9 2015,16:26:32)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_density_diffrn    1.770
_exptl_crystal_description       prism
_exptl_crystal_F_000             242
_exptl_crystal_size_max          0.20
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.17
_refine_diff_density_max         2.013
_refine_diff_density_min         -1.366
_refine_diff_density_rms         0.185
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.40(10)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.052
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     238
_refine_ls_number_reflns         3269
_refine_ls_number_restraints     33
_refine_ls_restrained_S_all      1.054
_refine_ls_R_factor_all          0.1014
_refine_ls_R_factor_gt           0.0892
_refine_ls_shift/su_max          0.013
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1300P)^2^+4.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2349
_refine_ls_wR_factor_ref         0.2484
_reflns_Friedel_coverage         1.000
_reflns_Friedel_fraction_full    0.945
_reflns_Friedel_fraction_max     0.862
_reflns_number_gt                2762
_reflns_number_total             3269
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            cm6b05249_si_006.cif
_cod_data_source_block           MHyMn100K
_cod_depositor_comments
'Adding full bibliography for 4002715--4002727.cif.'
_cod_database_code               4002721
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              79894
_shelx_hkl_checksum              38239